inplane shear behaviour of unreinforced masonry wallsktk.gf.ukim.edu.mk/documents/clenovi/sergey...
Embed Size (px)
TRANSCRIPT

Inplane shear behaviour of unreinforced masonry walls S. Churilov University Ss. Cyril and Methodius, Faculty of Civil EngineeringSkopje, Macedonia E. DumovaJovanoska University Ss. Cyril and Methodius, Faculty of Civil EngineeringSkopje, Macedonia ABSTRACT This paper presents the experimental testing and results of unreinforced masonry panels in order to obtain their behaviour under cycling loading. This study is part from an ongoing research programme. Mechanical properties of the constituent materials for masonry were tested and a database of characteristic properties was created. Several series of unreinforced masonry walls were constructed from solid clay bricks and lime mortar and tested under constant vertical load and cyclic horizontal loads. Later, strengthened masonry walls with reinforcedconcrete coating will be tested using the same geometry and boundary conditions. The purpose of the experimental investigations is to obtain the forcedisplacement curves, analyze the behaviour of masonry walls and establish design formulas for simple calculation of wall capacities for unreinforced and strengthened masonry walls. The results of the experiments will highlight the properties, advantages and limitations of the applied strengthening method. Keywords: masonry, shear, unreinforced, inplane, cyclic 1. INTRODUCTION In many seismically active regions around the world unreinforced masonry buildings represent a significant portion of the building stock. There is a large building stock of lowrise residential unreinforced masonry buildings in Macedonia and Balkan region. Their vulnerability is caused by the failure of unreinforced masonry shear walls due to the inplane or outof plane seismic loading. Large quantities of masonry structures do not satisfy the latest code provisions and therefore application of strengthening methods is necessary. This paper presents a part from an ongoing research for experimental and analytical investigation of strengthening and retrofit method applied to residential masonry buildings in Macedonia with a special attention on cost expenses, method for application and time for implementation. Macedonia is one of the most active seismic places in Balkan Peninsula, see Fig. 1. It lies in the south part of the Eurasian plate where three tectonic plates, African, Asian and European meet. It is mostly the work of African plate sliding beneath Eurasian plate that caused the geographic formation which we see today, and it is also the reason why there are frequent earthquake tremors in the region. The friction between the plates has brought about a number of fault lines which run across Macedonia approximately along the course of river beds. The one under Kochani along the river Bregalnica contributed to the 1904 earthquake, and the Skopje fault line along the river Vardar contributed to the 1963 earthquake which destroyed most of the city (Evans, 2007). Various techniques have been employed to strengthen and retrofit existing unreinforced masonry buildings. The conventional techniques such as posttensioning and adding steel reinforcements present complications in their application due to excessive time required for application, disruption of operations, corrosion of the steel and difficulties in handling of materials. In recent years, FRP materials have emerged as a promising alternative retrofit solution, with their lightweight, high strength, noncorrosive and electromagnetically inert properties, quick and easy application and with significant cost drops since their introduction in the early 1990s. One of the most used traditional techniques for strengthening existing residential masonry buildings in

Macedonia by improving its lateral resistance and energy dissipation capacity of the system is application of reinforcedconcrete coating (jacket) on one or both sides of the walls.
Figure 1. Seismic hazard map of Macedonia Figure 2. Earthquake damage on masonry building 2. EXPERIMENTAL TESTS ON MASONRY ELEMENTS In the present experimental study the testing of mechanical properties of bricks, mortar and masonry is performed according MKS codes and EN methods for testing. Three types of solid clay bricks, one type of hollow clay bricks and two mortar grades were tested to obtain mechanical properties. Three types of newly produced bricks from different manufacturers: Elenica (Asolid), Prilep (Bsolid) and KIK (Chollow) were used and one type was 5060 years old brick extracted from existing lowrise masonry building (Dsolid). All bricks have usual dimensions for this type of masonry elements with length, thickness and height of 250x120x65 mm. Hand made lime (LM) and cement mortar (CM) samples were tested with the following cement:lime:sand grades by volume: LM=0:1:3; CM=1:0:3. 2.1 Properties of bricks In order to understand the mechanical behaviour of a given material or structure, it is fundamental to perform experimental tests on it. In this way, it is possible to characterize its behaviour from the undamaged state through to peak and postpeak state. The properties of bricks were obtained by experimental testing according MKS B.D8.011:1987 standard. Table 1 summarizes the obtained results. The results show that series A and C deviate in small amount from the prescribed dimensions, while series B shows greater deviation. Series B shows greater surface unevenness and corner roundness in comparison with the other two series which leads to slightly lower unit weight. Series C results in lowest unit weight due to presence of holes through the unit. All brick types showed no visible failure after 5 cycles of freezing/unfreezing on temperatures ranging from 200C to +200C. Table 1. Physical properties of bricks Series Length
[mm] Width [mm]
Height [mm]
Weight in dry state [g]
Weight in saturated state [g]
Water absorption [%]
Weight after freezing [g]
Unit weight[kg/m3]
250,3 120,1 64,4 3721,0 4138,4 11,2 3719,9 1922,6B 241,1 120,9 64,5 3227,2 3692,7 14,4 3219,3 1719,9C 253,9 124,4 65,6 2565,4 2919,4 13,8 2556,9 1239,7
In order to obtain compressive and tensile strength, compression and tensile flexural tests were performed. According to this code compression tests were carried out on a series of 5 brick sandwich specimen made from 2 bricks glued with thin layer of cement mash, as shown in Fig. 3. Servocontrolled Interfels testing machine with load capacity of 3000 kN was used to test all brick specimens. Table 2 presents the obtained compressive strength with respect to brick type. For comparison of the obtained values for compressive strength another set of tests on cube samples with dimensions 50x50x50 mm extracted from the actual bricks was performed. The results from these tests presented in Table 3 showed higher values ranging from 1.5 to 2.3 times for each series.

Figure 3. Compression tests and failure mechanisms of solid clay bricks Table 2. Compressive strength of bricks according MKS standard
Series Compressive strength [MPa]
Series Compressive strength [MPa]
Series Compressive strength [MPa]
Series Compressive strength [MPa]
21 9,9 2B1 3,1 2C1 / (error in test) 2D1 9,9 22 13,1 2B2 4,3 2C2 7,7 2D2 3,5 23 7,3 2B3 2,6 2C3 6,9 2D3 6,6 24 12,0 2B4 4,6 2C4 6,4 2D4 6,1 25 11,9 2B5 5,5 2C5 4,7 2D5 4,4 Mean 10,8 Mean 4,0 Mean 6,4 Mean 6,1
Table 3. Compressive strength of bricks on cube samples
Series Compressive strength [MPa]
Series Compressive strength [MPa]
Series Compressive strength [MPa]
12 20,3 B11 7,1 D1 18,7 13 17,8 B12 9,4 D2 22,9 22 16,2 B22 8,2 D3 16,3 23 17,8 B23 11,0 D6 6,9 32 13,9 B32 8,7 D7 6,7 A33 12,2 B33 11,5 D8 6,5 Mean 16,4 Mean 9,3 Mean 13,0
Table 4 and Figure 4 present obtained values for brick tensile flexural strength and experiemntal failure mechanisms. Tensile strength was tested on a series of single bricks supported by steel roller bearings, simple beam system. Load was applied gradually through steel rod on top of the bricks acting like concentrated load. Table 4. Tensile strength of bricks
Series Tensile strength [MPa]
Series Tensile strength [MPa]
Series Tensile strength [MPa]
Series Tensile strength [MPa]
1 3,6 B1 1,6 C1 0,6 D1 3,0 2 2,2 B2 1,6 C2 0,9 D2 2,9 3 3,0 B3 1,5 C3 0,9 D3 2,4 4 2,8 B4 1,6 C4 1,0 D4 1,4 5 2,1 B5 0,9 C5 1,0 D5 4,6 6 2,8 B6 1,7 7 2,1 Mean 2,7 Mean 1,5 Mean 0,9 Mean 2,9
Figure 4. Tensile flexural tests and failure mechanism of solid clay bricks

2.2 Properties of mortars Parallel to the research done on the mechanical behaviour of solid clay specimens, this Section introduces a complementary experiment carried out on lime and cement mortar samples. The mortar types adopted in the tests were considered to reflect the most commonly used bonding material in existing buildings, lime mortars, and to compare it with the properties of stronger cement mortars. These tests were done according MKS U.M8.002:1968 standard on a 28 days aged samples with dimensions 40x40x160 mm. Table 5. Properties of mortar
Cement mortar Lime mortar Sample Unit weight
[kg/m3] Tensile strength [MPa]
Compressive strength [MPa]
Sample Unit weight [kg/m3]
Tensile strength [MPa]
Compressive strength [MPa]
1 20,2 1 0,5 1 2
2127,0 5,2 18,3
1 2 1385,3
0,08 0,5
3 19,5 3 0,6 2 4
1986,5 5,2 18,6
2 4 1367,0
0,10 0,5
5 36,7 5 0,6 3 6
2132,5 6,0 26,6
3 6 1391,9
0,19 0,7
7 24,7 7 0,5 4 8
2012,8 5,0 26,8
4 8
1367,7 0,10 0,5
9 21,4 9 0,5 5 10
2090,6 6,0 19,6
5 10
1409,0 0,08 0,6
11 25,1 11 0,5 6 12
2074,2 5,5 25,6
6 12
1380,0 0,05 0,6
13 26,4 Mean 1383,5 0,10 0,6 7 14
2140,2 5,7 26,8
15 37,1 8 16
2139,8 8,5 35,7
17 37,6 9 18
2083,3 6,7 37,8
Mean 2087,4 6,0 26,9
Figure 5. Experimental tests and failure mechanisms of mortar samples 2.3 Compressive strength of masonry Masonry compressive strength was tested on one wallet (UMWC1) with dimensions 120x120x25 cm and three wallets (UMWC2) with dimensions 52x32x12.5 cm build from solid clay bricks from series A and lime mortar with grading 0:1:3. The wallet UMWC1 was precompressed with load from the selfweight of the top RC beam. Load application was by manual with monotonic increasing of displacement increments while data acquisition was automatic. The test setup and results are presented in Fig. 6. Maximum vertical force measured was 705,6 kN at a displacement of 18,7 mm, which yields masonry compressive strength of 2,35 MPa. Initial modulus of elasticity is 200 MPa, while secant modulus is 50 MPa. Wallets denoted as UMWC2 were tested in axial compression according EN 10521:1998. Load application and data acquisition was automatic by Interfels testing machine. Figure 7 and Table 6 present wallet sample, failure mechanisms and obtained compressive strength.

UMWC1, Axial compression test ForceDisplacement (P)
0
100
200
300
400
500
600
700
800
0 2 4 6 8 10 12 14 16 18 20Vertical Displacement [mm]
Ver
tical
For
ce [k
N]
Fmax=705,6 kNu=18,7 mm
UMWC1, Axial compression test StressStrain ()
0,0
0,5
1,0
1,5
2,0
2,5
0,000 0,003 0,005 0,008 0,010 0,013 0,015 0,018Strain [%]
Stre
ss [M
Pa]
Figure 6. Compression test on wallet UMWC1
Table 6. Compressive strength of masonry wallets
Sample Maximum load V [kN]
Compressive strength f [MPa]
1 205,0 3,91 2 250,0 4,77 3 252,0 4,81 Mean f = 4,50
fk=f/1,2= 3,75
Figure 7. Compression test on wallets UMWC2 Using the equation 3.2 proposed in EN 199611:2005, determination of characteristic compressive strength of masonry for clay bricks of Group 1, fk=0,55fb0,7fm0,3, with normalized mean compressive strength of bricks from series A, Table 3 (=0,81), and compressive strength of lime mortar given in Table 5, one can obtain masonry compressive strength fk=2,35 MPa. If the normalized mean compressive strength of bricks from series A is taken from Table 2, then fk=1,76 MPa. When the compressive strength of bricks in not normalized with , then characteristic compressive strength of masonry is calculated as 2,73 MPa and 2,04 MPa, respectively. 2.4 Shear strength of masonry triplets Clay bricks from series A and lime mortar were used to prepare nine masonry triplets. The shear strength of masonry triplets was obtained as described in EN 10523:2002. Two load cells were used to carry out the shear tests, see Fig. 8. One load cell was used for monitoring the shear force and the other for monitoring compressive force acting perpendicular to the shear force. First, the desired compressive force was applied to the triplet and maintained constant during the test, while shear force was increased until the masonry triplet rupture occurred. Three precompressive stresses were adopted, as proposed in EN 10523, namely 0,2 MPa, 0,6 MPa and 1,0 MPa. The shear stresses obtained with the conducted tests are presented in Fig. 8. It also presents the linear regression as proposed in the standard. Triplets shear failure occurred mainly at mortar bed joints with predominant type of fracture A.1 as indicated in the standard.
fvoi = 1,3344  0,0494R2 = 0,9767
0,0
0,2
0,4
0,6
0,8
1,0
1,2
1,4
1,6
0,0 0,2 0,4 0,6 0,8 1,0 1,2
Precompression stress (MPa)
Shea
r st
ress
(MPa
)
Figure 8. Compression test on wallets UMWC2

3. EXPERIMENTAL TESTS ON MASONRY WALLS Many tests on masonry samples or small masonry walls have been performed, very often using diagonal compression loading to provide combined shear and compression load. To develop a suitable test setup it is essential to know how the shear stress is generated and distributed (Marzahn, 1998). The elastic theory, although strictly applicable to homogenous material can be used for uncracked masonry with certain reservations. The theory expresses that the shear stresses reach their maximum at a square element without prestressing at the centroidal axis, and the shear stresses generate principal stresses. The principal stresses, one compressive and the other tensile, are inclined by 450 to the longitudinal axis and the bed joint, respectively. Their values are equal to the shear stresses, see Fig. 9. It is assumed that the failure will occur if the principal tensile stress reaches the diagonal tensile strength of masonry covering both the sliding failure in bed joints and the cracking of units. Similar to this arrangement a rectangular shaped wall is formed with a length of 2,6 m, and height of 1,8 m thus reaching the limitations of the testing frame. First, vertical loading is applied and kept constant during testing and then horizontal displacement increments are cyclically applied on the top RC beam. Displacements are measured in several points using displacement transducers. The experimental setup is shown in Fig. 11. Several tests were carried out to evaluate the shear resistance of unreinforced masonry walls. In this paper only results of two tests are presented, see Fig. 12.
Figure 9. Homogenous element
subjected to pure shear
15
10
5
0
5
10
15
0 5000 10000 15000 20000 25000 30000
Time (s)
Dis
plac
emen
t (m
m)
measuring device D2front
Figure 10. Displacement history Figure 11. Test setup for shear tests of masonry walls
Unreinforced masonry walls from solid clay bricks (series A) and lime mortar with dimensions 260x180x25 cm (UMW1) and 150x180x25 cm (UMW2) were constructed and tested with vertical precompression stress of 1,0 MPa. UMW1 reached maximum resistance of 213,2 kN at corresponding displacement of 6,74 mm and ultimate displacement of 12,2 mm. For wall UMW2 maximum obtained resistance was 99,13 kN at displacement of 7,35 mm and ultimate displacement of 17,24 mm. From Figure 12 it is possible to observe a global behaviour characterized by energy dissipation and some ductile behaviour. UMW2 showed greater ductility than UMW1 with expected lower maximum resistance and slowly decreasing softening branch as presented by hysteresis envelopes.
250
200
150
100
50
0
50
100
150
200
250
20 15 10 5 0 5 10 15 20
Displacement (mm)
Shea
r fo
rce
(kN
)
Forcedisplacement hysteresisHysteresis envelope
250
200
150
100
50
0
50
100
150
200
250
20 15 10 5 0 5 10 15 20
Displacement (mm)
Shea
r fo
rce
(kN
)
Forcedisplacement hysteresis
Hysteresis envelope
Figure 12. Typical lateral displacementlateral resistance hysteresis loops for walls UMW1 and UMW2

Both walls failed with combination of shear and compression failure with head and bed joint failure and brick failure, as shown in Fig. 13.
Figure 13. Observed failure mechanisms and crack propagation for walls UMW1 and UMW2
3.1 Masonry resistance to lateral loads When a masonry building is subjected to a ground motion, the resisting elements may have three different failure modes in their plane: sliding shear, diagonal shear cracking and flexure. Sliding shear failure mode usually occurs for a low level of axial load and poor quality mortar, causing the sliding of an upper part of the wall on one of the horizontal joints. As reported by Tomaevi (1999), it usually happens in the upper floors of buildings, where vertical loading acting on the wall is low but accelerations are high because of the shape of the seismic response of a masonry building. The sliding shear resistance is given by Eq. (1).
( )0 += vosl ftLH (1) where L is the length of the wall, t is the thickness, fvo is the initial shear strength under zero compressive strength, is the contribution of compression stresses (usually 0,10,4), 0 is the compression stress perpendicular to shear. Diagonal shear cracking is the common masonry failure mode under seismic loads and happens for a combination of vertical and horizontal loads where the principal tensile stresses developed in the wall due to this action exceed the tensile strength of masonry. The formulation of the maximum lateral resistance of a wall falling in diagonal shear cracking is presented by Eq. (2).
( )511110 ,b,Lhb,
fbfAH
t
tsdc =+=
(2)
where A is the horizontal crosssection area of the wall, ft is the tensile strength of masonry, b is the shear stress distribution factor, depending on the geometry of the wall and N/Hmax ratio. Flexural resistance of unreinforced masonry is conditioned by crushing of the compressive part. Considering the behaviour of masonry subjected to uniaxial compression similar to that of concrete, with a similar shape of an equivalent rectangular stress block, the flexural resistance can be calculated by using Eq. (3).
hf
Lt
H fl
=
02
0 12
(3)
where f is the compressive strength of masonry and is coefficient which defines position of the moment inflection point along the height of the wall. If the design capacity is correlated with design actions then in Eq. (3) design value of compression stress d, characteristic value of compressive strength of masonry fk and partial safety factor for masonry m should be considered. Equations (1), (2) and (3) are used to predict the maximum load and failure modes of walls UMW1

and UMW2 for uncracked wall section. Adopted compressive strength is given in Table 6, while tensile strength is taken as 0,05compressive strength and compression stress perpendicular to shear is 1,0 MPa. The results from those calculations are compared with experimentally obtained values and shown in Table 7 and Fig. 14. Table 7. Predicted and experimental maximum resistances
Predicted Experimental Failure/Resistance UMW1 UMW2 UMW1 UMW2
Sliding shear [kN] 266,50 263,75 Diagonal shear [kN] 278,83 187,54 Flexure failure [kN] 688,52 291,30
213,2 99,13
Figure 14. Predicted vs. Experimental results 4. CONCLUSION This paper presents a research into experimental investigation of the behaviour of inplane loaded unreinforced masonry panels and the results of the experiments carried out. Although this research is currently in progress, this study demonstrates the behaviour of unstrengthened URM walls under cyclic loads, shows damage propagation and failure mechanisms, horizontal loaddisplacement hysteresis behaviour and diagrams, identification of the characteristic limit states, stiffness degradation and energy dissipation. Furthermore, the investigations will be enlarged with experimental testing of strengthened masonry panels with RC jacketing to compare with the behaviour of plain masonry walls. ACKNOWLEDGMENTS The authors acknowledge factory for clay bricks and blocks Elenica, Strumica for supplying solid clay bricks used in the tests, University Ss. Cyril and Methodius, Faculty of Civil EngineeringSkopje for help in preparation and execution of laboratory tests, ADING AD for supplying admixtures for test setup, Factory Karpos for providing RC beams and University Ss. Cyril and Methodius, Faculty of Mechanical Engineering for contribution in data acquisition during experimental tests. REFERENCES Evans, T. (2007). Macedonia: The Bradt Travel Guide, Edition: 2, illustrated. Published by Bradt Travel Guides. MKS B.D8.011 (1987). Testing methods of clay bricks, blocks and slabs. MKS U.M8.002 (1968). Mortars for masonry and plastering. Testing methods. CENEN 10521 (1998). Methods of tests for masonry  Part 1: Determination of compressive strength. CENEN 199611 (2005). Eurocode 6  Design of masonry structures  Part 11:General rules for reinforced and
unreinforced masonry structures. CENEN 10523 (2002). Methods of test for masonry  Part 3:Determination of initial shear strength. Marzahn, G. (1998). The Shear Strength of DryStacked Masonry Walls. LACER No. 3, 247262. Tomaevi, M. (1999). EarthquakeResistant Design of Masonry Buildings, Series on Innovation in Structures
and Construction, Vol. 1, Imperial College Press, London. Tomaevi, M., Klemenc, I., Lutman, M., (2000). Strengthening of existing stonemasonry houses: lessons
learned from the earthquake of Bovec of April 12, 1998, European Earthquake Engineering, 1, 1322.
Dominant failure mode is marked in grey cells. Difference in prediction vs. experimental results: UMW1 30,6 %; UMW2 89,2 %
0
50
100
150
200
250
300
0 1 2Wall
Max
imum
res
ista
nce
[kN
]
PredictedExperimental